2012 Gong and Wu, licensee InTech. This is an open access chapter distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/3.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Novel Polyimide Materials Produced by Electrospinning
Guangming Gong and Juntao Wu*
Additional information is available at the end of the chapter
Due to one-dimentional nanostructures unique properties and their intriguing applications, there has being a great demanding on the technologies which are able to produce such structures. Among the applicable strategies, electrospinning seems to be the simplest approach to generate continues nanofibers with ultrathin and uniform diameters (Li & Xia, 2004). Electrospinning is a spin technology which involves the use of a high voltage, usually direct-current, to trigger the formation of a liquid jet (Li & Xia, 2004; Greiner & Wendorff, 2007).
1.1.1. The Mechanism of Electrospinning
Briefly, the mechanism of electrospinning is often to be explained as the collaborative effects of electrostatic repulsion by the accumulated charges on the surface of polymer solution and the Coulombic force exerted by the external electric field (Li & Xia, 2004; Greiner & Wendorff, 2007). A illustrative figure may help the understanding of it. As can be seen in Figure 1, polymer solutions are added in a syringe with a metal spinneret connected on its tip. Driven by a syringe pump or gravity, the solution starts to flow out. When a high voltage (usually in the range from 1 to 30 kv), the pendent drop of the solution will be highly electrified. During this process, the liquid drop will be shaped into a cone-like object, as known as Taylor Cone. And the charges on the surface will repulse each other, overcome the surface tension of the solution until reaching a certain threshold. Then an ejection of solution is formed. Driven by the mighty electric field, the liquid jet undergoes a mighty stretching force, elongating the jet, thinning the diameter to a certain range. While during this period, the solvent evaporates intensively. Thus, the electrospun polymer fibers are formed. And a typical SEM photo of the electrospun fiber is illustrated in the insert of
High Performance Polymers Polyimides Based From Chemistry to Applications 128
Figure 1. Electrospinning is able to produce fibers whose diameters ranged from tens of nanos to a few microns. And a great amount of polymers are reported to be successfully spun into fibers via this technology. Based on the experimental data and electrohydrodynamic theories, several groups have built mathematical model to describe behaviors of electrospinning. Further information is not explained here, if interested, one can refer to these literatures: (Reneker, Yarin & Fong, et al., 2000; Yarin, Koombhongse & Reneker, 2001; Hohman, Shin & Rutledge, et al., 2001, etc.)
Figure 1. An illustration of a typical electrospinning set and the formation of the liquid jet (in enlargement). The inserted is an SEM picture of nowoven PI mat prepared in our laboratory.
1.1.2. A Brief History of Electrospinning
The first patent that describe the operation of electrospinning appeared in 1934 (Formalas, 1934), when Formalas disclosed an apparatus for producing polymer filaments by taking the advantage of electrostatic repulsions between surface charges. It has been almost 80 years since the patent but electrospinning existed only as a theory in peoples mind until 1990s. (Li & Xia, 2004) During that period, there were only few reports on ES. Its value was not fully attended so that no further development was made. But in the beginning of 1990s, by the efforts of several research groups, especially the ones leaded by Prof. D. H. Reneker and Prof. G.C. Rutledge, people demonstrated that ES was able to produce a great amount of polymer fibers. A large campaign of polymer ES researches was waged. (Wikipedia, Online) The timely demonstrations popularized the term electrospining in literatures that we see today.
1.1.3. Development and Applications
The diameters of polymer fibers produced by electrospinning were able to reach an incredible small range. Compared to traditional polymer fibers, ES fibers have greater
Novel Polyimide Materials Produced by Electrospinning 129
specific areas and aspect ratio (Li & Xia, 2004; Greiner & Wendorff, 2007). Electrospinning is a method to produce not only pure fiber structures, but also many other morphologies. By tuning electrospinning parameters (e.g. electric field strength, viscosity of spinning solution, solvents, etc.) and/or choosing different ES methods, controllable morphologies of ES products can be achieved. Owing to the world wide collaborative efforts, so far, people are able to electrospin pearl-necklace-like beaded fiber structures (Greiner & Wendorff, 2007), highly porous fiber structures (Bognitzki et al., 2001), grafted fiber structure (Hou H, Reneker D H, 2004; Chang Z, 2011), hollow interior micro tubes (Li, Wang & Xia, 2004; Zhao, Cao & Jiang, 2007), wire-in-tube structures (Greiner & Wendorff, 2007), Whats more, twisted fiber bundles, golfball-like micro particles and multi-chambered hollow spheres (Chen et al., 2008) are also able to be generated via this technique. These fibrous structures and particles obtained by electrospinning have some unmatchable properties, like the
Figure 2. Morphologies of electrospun products: a) pear-necklace like fibers. Copyright 2007 WILEY-VCH, reused with permission; b) highly porous fibers. Copyright 2001 WILEY-VCH, reused with permission; c) grafted fibers. Copyright 2004 WILEY-VCH, reused with permission; d) a bundle of electrospun PI micro rope (Gong & Wu, unpublished work); e) wire-in-tube fibers. Copyright 2007 WILEY-VCH, reused with permission; f); aligned micro tubes. Copyright 2004, American Chemical Society, reused with permission; g) multi-channel tubes. Copyright 2007, American Chemical Society, reused with permission; h) golfball-like spheres (Gong & Wu, unpublished work); i)multi-chamber spheres. Copyright 2008, American Chemical Society, reused with permission
High Performance Polymers Polyimides Based From Chemistry to Applications 130
extremely long length, high surface area, complex pore structure, alignment on the molecule level, etc. Such properties enable the electrospun materials possessing the potential values in applications and research fields, e.g. templates, filter and textile, catalysis and enzyme carriers, nanofiber reinforcement, medical applications, and surfaces with special wettability, etc. Due to the space constraints, detailed instances are not discussed here. The further introductions and examples, if one is interested, can be reffered to these literatures: (Li & Xia, 2004; Greiner & Wendorff, 2007; Lu, Wang & Wei, 2009)
1.2. Polyimide (Ding, 2011)
Polyimide (PI) is a polymeric material which contains imide rings in their molecule backbones. PI is mainly obtained through a two-step method: fragrant diamine and dianhydride undergo a condensational polymerization and then a thermal/chemical imidization, to afford PI, illustrated in Figure 3. The representative PI is Kapton, developed and commercialized by Dupont in 1960 and 1965, respectively. This golden film presents good mechanical properties and high thermal stability. After 50 years, Kapton is still a leading material in thermal tolerable materials. After Kaptons success, a series of fragrant polyimides were developed and accepted by the market. PIs wide popularity is due to its comprehensive performances: wide applicable temperature range, good mechanical, electrical properties and bio-compatability. Besides, PIs broad molecular designing window also guarantees its rapid development: by modifying molecular structures of diamine and dianhydride, different kinds of soluble and thermal shapeable PI were prepared. After a long term of research and developing state, PI is now extensively employed in the aerospace and aviation industries and in the microelectronic and electric fields as advanced packaging and insulating materials. With the rapid development of these advanced industry, novel PI materials with high performances and new functions are usually required.
O + Ar NH2H2N ArC
Thermal or ChemicalImidization
Figure 3. A two-step PI synthetic route
Novel Polyimide Materials Produced by Electrospinning 131
1.3. Electrospun polyimide materials
In 1996, Reneker referred that PI nano fibers are obtainable via electrospinning (Reneker & Chun, 1996). In 2003, Nah et al. described in details the method to produce PI nano fibers (Nah, Han & Lee, 2003), declared the successful preparation of ultra-thin PI fibers. The morphology of the PI fibers is shown in Figure 4. The successful preparation was a milestone that it was when a polymer with comprehensive high performances encountered a versatile and effective method for fiber producing. Their combination afforded a series of results with both scientific amd industrial values. Herein, this chapter summarized and categorized the works of electrospun PI materials since 2003. In the meantime, some outlooks of this research field were also given.
Figure 4. Nah et al. obtained PI fibers by electrosp